ISSN: 0973-4945; CODEN ECJHAO
E-Journal of Chemistry
http://www.e-journals.net 2010, 7(3), 1090-1094
Influence of Benzotriazole on Corrosion Inhibition of
Mild Steel in Citric Acid Medium
P. MATHESWARAN* and A.K. RAMASAMY
*Department of Chemistry, Vidyaa Vikas College of Engineering and Technology,
Tiruchengode, Namakkal Dt. -637 214, India.
Department of Chemistry, Periyar University, Salem Dt., India.
Received 6 November 2009; Accepted 2 January 2010
Abstract: Benzotriazole an organic compounds has been studied as corrosion
inhibition for mild steel in 1 N citric acid by weight loss method. The result
showed that the corrosion inhibition efficiency of the compound was found to
be varying with the temperature and acid concentration. Also it was found that
the corrosion inhibition behaviour of benzotriazole is better when the
concentration of inhibitor is increased. The kinetic treatment of the results
shows first order kinetics.
Keywords: Mild steel, Corrosion Inhibitors, Weight loss method and Benzotriazole.
Iron and its alloys are extremely used in many engineering application in various
environments especially in inorganic and organic acid environments because of their
excellent combination of properties1-2
. Various types of inhibitors have been used as
corrosion inhibitors for mild steel corrosion in acidic medium3. High electron density of the
sulphur and nitrogen atoms in the heterocyclic organic compounds helps the organic
molecules to get chemisorbed on to the metal surface4. Most of the earlier studies have been
related to the general performance and the inhibition of mild steel corrosion in organic acid5-6
So in this investigation the corrosion behoviour of mild steel in 1 N citric acid medium in
the absence and presence of benzotriazole at various temperature by weight loss method.
According to ASTM method7 as reported already cold rolled mild steel strips were cut into
pieces of 5 cm 1 cm having the following composition (in percentage) of Fe = 99.686, Ni
= 0.013, Mo = 0.015, Cr = 0.043, S = 0.014, P = 0.009, Si = 0.007, Mn = 0.196 and C = 0.017.
Concentration of Benzotriazole
Concentration of Benzotriazole
Influence of Benzotriazole on Corrosion Inhibition 1091
They were pickled in pickling solution (5% H2SO4) for 3 minutes and washed with distilled
water followed by polished with various grades of emery papers and degreased using
trichloroethylene. The weight of specimen were noted and then immersed in test solution
containing various concentrations of inhibitors at room temperature 303K, 353K and 403K.
After the duration of 2 h in citric acid, the specimens were removed from test solutions and
pickled in pickling (5% sulphuric acid) solution, dried and finally weighed. The differences
in weights were noted and the corrosion rates were calculated.
All the solutions were prepared using NICE brand AR grade chemicals in double distilled water
and bubbling purified by nitrogen gas for 30 minutes to carry out de-aeration of the electrolytes.
Citric acid solution was prepared by double distilled water. The corrosion inhibitor solution of
0.1 % benzotriazole was prepared by dissolving 1 g of benzotriazole in 100 mL of test solution.
And also, 0.2%, 0.3%, 0.4% and 0.5% solutions of benzotriazole were prepared.
Results and Discussion
The corrosion behavior of mild steel in citric acid (Figure 1) and analyzed by weight loss
method at different temperatures (303K, 353K and 403K).
Figure 1 (a). Variation of corrosion rate (CR) with concentration of benzotriazole (in %) in
citric acid solution at different temperature,
Figure 1(b). Variation of inhibition efficiency (IE) with concentration benzotriazole (in %)
in citric acid solution at different temperature.
1092 P.MATHESWARAN et al.
From the graph, it was observed that the weight loss of mild steel in the acid decreases
with increasing concentration of additives, which suggesting that the additives are corrosion
inhibitor for mild steel in 1 N citric acid. From the data of weight loss method, the corrosion
rate (CR) was calculated using the equation:
CR= (87.6 x W) / (D x A x T)
W, D, A and T are weight lose (in mg), density of mild steel (7.86 g/cc), area of the
specimen in cm square and exposure time in hours respectively. Similarly, Inhibition
efficiency was calculated using the equation,
IE % = [(WoWi)/Wo] x 100
Wo and Wi are the values of the weight loss (in g) of mild steel in the absence and
presence of inhibitor respectively. The values of corrosion rate and inhibition efficiency in
absence and presence of difference concentration of inhibitor used in 1 N citric acid solution
at 303, 353 and 403K for 2 h were given in Table 1.
Table 1. Corrosion inhibition behaviour of mild steel in 1N citric acid solution in absence
and presence benzotriazole by weight loss measurement.
Corrosion rate,mm/y Inhibition Efficiency, % Corrosion
inhibitor, % 303K 353K 403K 303K 353K 403K
Blank 20.84 680.04 858.81 - - -
0.1 13.59 474.67 624.68 41.57 39.15 34.85
0.2 9.81 418.94 568.73 50.56 46.29 41.84
0.3 8.13 367.34 513.01 69.10 52.91 46.49
0.4 5.57 306.49 432.76 76.97 60.71 57.18
0.5 4.12 249.87 377.04 79.21 67.97 60.67
From Table 1, it is evident that, the corrosion rate was decreased with increasing
concentration of inhibitor and inhibition efficiency increased with increasing the
concentration of the inhibitor. In addition, the maximum corrosion inhibition efficiency of
benzotriazole was increased 0.1% to 0.5%. Also the inhibitor efficiency is compared at 0.5%
concentration the rate of efficiency is high at 303K when compared to 403K respectively in
1 N citric acid. And also, it was concluded that benzotrizole was best inhibitor in mild steel
corrosion in citric acid medium at low temperature.
In addition, the experiment was conducted at different immersion time to study the rate of
reaction. The plot of log (weight loss) versus immersion time as shown in Figure 2, gave a
straight line indicating that it follows first order reaction. The values of the rate constant was
calculated using the first order rate law,8 k = (2.303/t) log ([Ao]/[A]). Here [Ao] is the initial
mass of the metal and [A] is the mass corresponding to timet.
The half-life (t1/2) were calculated using the relationship,9 t1/2 = 0.693 / k. The values of
rate constant and half-life (t1/2) obtained from the above relations were summarized in Table 2.
Half life values were found to be constant at different immersion time. The constant value of
the rate constant further confirmed that the corrosion of mild steel in Citric acid solution in
presence of benzotriazole follows first order reaction.
Influence of Benzotriazole on Corrosion Inhibition 1093
Figure 2 (a). Half life plot for weight loss with immersion time in citric acid solution in the
presence of benzotriazole at 303K.
Figure 2 (b). Half life plot for log (weight loss) with immersion time in citric acid solution
in the presence of benzotriazole at 303K.
Table 2. Rate of constant (k) and half-life values for the corrosion of mild steel at different
immersion times in 1 N citric acid solution in absence and presence of inhibitors of different
concentration at 303K.
Inhibitor, in %
k (x 10-3
0.1 1.760595( + 0.059) 393.6
0.2 1.578338( + 0.042) 439.1
0.3 1.582695( + 0.033) 437.9
0.4 1.362773( + 0.016) 508.5
0.5 1.248923( + 0.011) 554.9
1094 P.MATHESWARAN et al.
Corrosion inhibitory behaviour of benzotriazole
Since hydrazinecarboxamide groups are basic in nature due to availability of electrons on N
atom, it acts as adsorption center. Hence, benzotriazole shows goods inhibitory character.
Hence the N atom in benzotriazole therefore undoubtly has high electron density for
adsorption on to the mild steel surface. So, inhibition behaviour of benzotriazole increases
The benzotriazole showed good performance as corrosion inhibitor in Citric acid solution
medium due to the presence of heteroatom and unsaturated bond that cause effective
adsorption process leading to the formation of an insoluble protective surface film which
suppresses the metal dissolution reaction. First order types of reaction were observed in the
kinetic studies. The inhibition efficiency increased with increase in concentration of
inhibitors for 0.1% to 0.5% and decreased with rise in temperature from 303K to 404K. The
maximum inhibition efficiency of benzotriazole were 41.57% and 79.21% respectively in 1 N
Citric acid at 303K [0.5%] for 2 h of immersion tim